Nanostructurization of Fe-Ni Alloy
© The Author(s). 2017
Received: 26 December 2016
Accepted: 2 March 2017
Published: 17 March 2017
Data about an effect of cyclic γ-α-γ martensitic transformations on the structure state of reverted austenite Fe-31.7 wt.% Ni-0.06 wt.% C alloy are presented. The effect of multiple direct γ-α and reverse α-γ martensitic transformations on fragmentation of austenitic grains has been investigated by electron microscopy and X-ray diffraction methods. An ultrafine structure has been formed by nanofragmentation inside the initial austenite grains due to the successive misorientation of their crystal lattice. Austenite was nanofragmented as a result of multiple γ-α-γ martensitic transformations. Slow heating of the nanofragmented alloy at a rate below 2 °C/s results in nanograin refinement of the structure by multiplication of the reverted γ-phase orientations. The conditions of structure refinement up to ultrafine and nanocrystalline levels as a result of both shear and diffusion mechanisms of reverse α-γ transformation are determined.
KeywordsAustenite Martensitic transformation Nanofragment Phase hardening Thermocycling
PACS68.35.bd Metals and alloys 68.35.Rh Phase transitions and critical phenomena 68.37.-d Microscopy of surfaces, interfaces, and thin films
Compacted nanocrystalline metallic materials can be produced by the methods of powder metallurgy and intensive plastic deformation (IPD) [1, 2]. These materials including those having practical importance possess special structure, which provides their unique properties. Nevertheless, the methods mentioned are technologically complicated and energy-consuming. Moreover, the IPD methods are applicable only for thin disc fabrication. These drawbacks are overcome in the approach, which involves refinement of the crystalline structure by the cyclic γ-α-γ (fcc-bcc-fcc) martensitic transformations. The refinement occurs in the process of the reverse α-γ transformation whereby ultrafine or nanocrystalline reverted austenite is formed [3–7]. The structural refinement can be regarded as an extension of the method of austenitic alloy hardening by the reverse α-γ transformations that were firstly developed at Institute of Metal Physics of NASU (Kyiv, Ukraine) and referred to the method of phase hardening .
This paper introduces a procedure used for refinement of the Fe-Ni alloy to nanoscale level by the cyclic direct γ-α and reverse α-γ transformations.
The subject of this study was metastable Fe-31.7 wt.% Ni-0.06 wt.% C alloy, which was in the austenitic state at room temperature. The direct γ-α transformation occurred when cooling in liquid nitrogen. The reverse α-γ transformation occurred after heating at the rate of 70 °C/s of the samples up to 400 °C in a salt bath (55% NaNO3 + 45% KNO3). The phase transition kinetics was studied using differential magnetometry . Characteristic temperatures of the γ-α and α-γ transformations were determined by magnetization measurements. The X-ray analysis was carried out on single crystalline samples. To prepare a coarse crystalline ingot in a high-frequency induction furnace, a melt has been slowly cooled down to temperature of 1050 ÷ 1100 °C and then was quenched in salt water. The cylindrical single crystals were cut from coarse grains for the X-ray measurements.
The X-ray diffractometry of single crystalline samples was performed in RCW-86 rotation chamber with photo registration using FeKα radiation. Single crystals were employed to provide an observation of crystal lattice misorientation in the range from a fraction of a degree to several tens of degrees, i.e., to observe the development of the structural fragmentation. The maximum misorientation angle ψ, which characterizes the degree of the structural fragmentation, was determined from the azimuthal smearing of the (200)γ and (002)α reflections of the reverted austenite and the martensite. Microstructure was investigated using automatic structure analyser (Epiquant, Germany), transmission electron microscope (TEM) Philips CM-10, and scanning electron microscope (SEM) Jeol JSM-6490-LV (BCE mode).
Results and Discussion
The ability of austenite to produce the fine structure due to formation of highly dispersed fragments in the process of cyclic martensitic transformations was demonstrated in the work . In this study, austenite recrystallization of nickel-iron alloys after the multiple γ-α-γ transformations (α-γ ones being diffusionless) was firstly described.
The X-ray diffraction pattern of single crystalline specimens demonstrated the azimuthal smearing of the austenite reflections after the reverse α-γ transformation. With increase of the number of cycles, the magnitude of ψ was increased and diffraction spots embedded in Debye rings progressively became more smeared along the azimuthal direction. After 80–100 γ-α-γ transformations, the diffraction pattern contained the reflections of the reverted austenite, which was significantly smeared out along the azimuthal direction up to 16°. The γ- and α-phase reflections underwent different extent of azimuthal smearing depending on the degree of crystalline fragmentation. The misorientation of the γ phase was higher than that of the α phase indicating suppression of the martensitic transformation in the most misoriented fragments of the reverted austenite.
A considerable number of 200–800-nm fragments was observed after 30 cycles. After 60–100 cycles, their sizes were reduced to 70–100 nm.
Our investigations have shown that in nickel-iron alloys, the fragmentation of initial austenite to nanoscale size (nanofragmentation) occurs if the reverse α-γ transformation is diffusionless.
Structural state of the reverted austenite is formed in the process of the multiple reverse diffusionless α-γ transformations and following α-γ transformation controlled by diffusion mechanism. Diffusionless mechanism of reverse α-γ transformation of the investigated alloy occurs at the heating of quenched alloy in the interval of this α-γ transformation with critical rate 70 °C/s. The small amount of carbon up to 0.1 wt.% was not changed of the critical rate of heating.
Additional alloying of Fe-Ni austenite by carbon can increase the grinding degree of reverted austenite in the process of the reverse α-γ -transformation [10–13]. Thermal cycling without γ-α-γ transformations do not result in significant refinment of initial structure [14, 15].
The mechanism involving the formation of highly dispersed nanoscale level structures by cyclic martensitic transformations can be employed for development of metastable alloys with improved physical and mechanical properties.
The fragmentation of the reverted austenite can occur in the Fe-31.7 wt.% Ni-0.06 wt.% C alloy in the process of the cyclic γ-α-γ transformations due to development of the misorientation processes in the crystal lattice. The cyclic γ-α-γ transformations led to the formation of fragments of nanoscale size; after 80–100 cycles, most of the fragment size was from 70 to 100 nm.
Slow heating of the quenched alloy at a rate below 2 °C/s results in nanograin refinement of the structure by multiplication of the reverted γ-phase orientations. Initially, the nanofragmented structure of the austenite must be formed by the cyclic γ-α-γ transformations. The orientation multiplication takes place due to the diffusion mechanism of the reverse α-γ transformation.
In contrast to the method of the phase hardening, which was earlier used only for hardening, the method of structural refinement by cyclic martensitic transformations is highly promising technique not only for hardening but also for improvement of physical (e.g., magnetic, diffusion, shock-proofing) properties of metastable alloys.
Intensive plastic deformation
The author thanks P. Volosevich and V. Bondar for participating in the experiments.
The author declares that he has no competing interests.
Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
Open AccessThis article is distributed under the terms of the Creative Commons Attribution 4.0 International License (http://creativecommons.org/licenses/by/4.0/), which permits unrestricted use, distribution, and reproduction in any medium, provided you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made.
- Gleiter H (2000) Nanostructured materials: basic concept and macrostructure. Acta Mater 48:1–29View ArticleGoogle Scholar
- Valiev RZ, Alexandrov IV (2000) Nanocrystalline materials. Logos, MoscowGoogle Scholar
- Kessler H, Pitsch W (1967) On the nature of the martensite to austenite reverse transformation. Acta Met 15:401–406View ArticleGoogle Scholar
- Sagaradze VV, Kabanova IG (1999) Formation of nanocrystalline structure during direct and reverse martensitic transformations. Mater Sci Eng 273–275:457–461View ArticleGoogle Scholar
- Nedolya AV, Shapar DY (2016) Estimation of energy of cubic iron-carbon nanoclusters by molecular mechanic method. Mater Werkst 47(2-3):128–132View ArticleGoogle Scholar
- Sagaradze VV, Danilchenko VE, L’Heritier P, Shabashov VA (2002) The structure and properties of Fe-Ni alloys with a nanocrystalline austenite formed under different conditions of gamma-alpha-gamma transformations. Mater Sci Eng 337:146–159View ArticleGoogle Scholar
- Danilchenko VE, Sagaradze VV, Dzevin IM (2013) Effect of multiple martensitic transformations on structure of Fe-Ni alloys. J Mater Sci Technol 29(3):279–282View ArticleGoogle Scholar
- Malyshev KA, Sagaradze VV, Sorokin IP et al (1982) Phase-transformation-induced hardening of iron-nickel-based alloys. Nauka, MoscowGoogle Scholar
- Bondar VI, Danilchenko VE (1984) Influence of phase cold working on the structure and strengthening of iron-nickel single crystals. Reports of USSR Academy of Sciences 275:1408–1412Google Scholar
- Nedolya AV, Bondarenko NV (2016) Change of energy of the cubic subnanocluster of iron under influence of interstitial and substitutional atoms. Nanoscale Res Lett 11:15View ArticleGoogle Scholar
- Nedolya A (2016) Conditions of spontaneous growth of iron subnanocluster: the influence of impurity atoms. In: Book, Fesenko O, Yatsenko L (eds) Nanophysics, nanophotonics, surface studies, and applications, Springer International Publishing Switzerland 2016; Springer Proceedings in Physics, vol 183., pp 231–245Google Scholar
- Nedolya AV (1997) XRPD application for laser-treated surface of Fe-based alloys study. Il Nuovo Cimento D 19(2-4):609–615View ArticleGoogle Scholar
- Dzevin IM (2015) Microstructure inhomogeneity of Fe-31% Ni alloy and stabilization of austenite. Nanoscale Res Lett 10:117View ArticleGoogle Scholar
- Bazeluk GY, Bondar VI, Dzevin YN (2007) X-ray diffraction investigations of crystallic structure changes in the Ni-based alloy at the thermal cycling. Solid State Phenom 130:267View ArticleGoogle Scholar
- Andryushchenko VA, Gnatyuk IY, Dzevin EN, Shapoval TA (2001) Getting the special properties of the Fe-Al-C Alloys by means of inducing of phase and structural changes. Metal physics and new technologies 23:257–261Google Scholar